Scandinavian Journal of Metallurgy 2003; 32: 15–32 Copyright C© Blackwell Munksgaard 2003 Printed in Denmark. All rights reserved SCANDINAVIAN JOURNAL OF METALLURGY ISSN 0371-0459 An investigation of slag floatation and entrapment in a continuous-casting tundish using fluid-flow simulations, sampling and physical metallurgy Henrik Solhed1,2 and Lage Jonsson1,3 1MEFOS, Lulea˚; 2Department of Physics, Lulea˚ University of Technology; 3Department of Materials Science and Engineering, KTH, Stockholm, Sweden Some aspects of inclusion behaviour in the tundish have been investigated both theoretically and experimentally. Good agreement was obtained between measured and predicted temperature and flow fields for 1- to 6-strand continuous- casting tundishes. In this study the flow field was redesigned with weirs, resulting in the addition of a vertical component to Stoke’s equation. The results indicate an increase in the velocity that cause a rise of inclusions (smaller inclusions (<20 µm)). Consideration of slag, flux and refractory in the model has also made it possible to simulate the mixing of steel and slag. Special sampling techniques were used to gather information. Samples were analysed using ultrasonic testing, LOM, SEM and Atomic Force Microscopy (AFM). The analysis results were used to verify the predictions regarding steel/slag mixing and understanding of physical conditions at the inter- faces. As a result, the casting praxis was improved (cleaner steel) and the products were of higher quality. Key words: clean steel, fluid flow, microscope studies, mix- ing, models, sampling, slag, steel, theory, tundish. C© Blackwell Munksgaard, 2003 Accepted for publication 24 May 2002 Extensive efforts have been made in academia and industry over the past decades to exploit and en- hance continuous-casting-tundish systems with respect to their metallurgical performance. As a consequence, numerous physical and mathematical modelling studies embodying both industrial and water-model tundishes have been carried out and reported in the literature. Recently, Mazumdar & Guthrie  reviewed these modelling efforts of continuous-casting systems. They pointed out that a modern-day steel-making tundish should be designed to provide maximum opportunity for carrying out various metallurgical operations such as inclusion separation, flotation, alloy trimming, inclu- sion modification, superheat control, as well as ther- mal and particulate homogenisation. Furthermore, they concluded that mathematical studies indicate that flow conditions conducive to the removal of non-metallic inclusions from tundishes can be created by inserting appropriate flow-modification devices. The optimal de- sign and location of flow modifiers, with respect to clean steel, clearly depend on tundish geometry , the oper- ating conditions and very much on the steel inclusions’ size range. In the models reported on, however, the refractory has rarely been included and, to the knowledge of the authors, neither the flux nor liquid slag have so far been included in any modelling efforts. It is obvious though that both the refractory and the slag layer preferably should be the integrated parts of the model for appro- priate understanding of many metallurgical issues such as thermal and inclusion behaviour because the slag and the refractory are both potential sources, sinks and mod- ifiers for inclusions. Furthermore, a useful approach to modelling fluid flow in the slag phase enables studies of heat and fluid-flow conditions coupled with thermo- dynamics in the very important steel/slag region (from a metallurgical point of view) in a continuous-casting tundish. The alternative of coupling fluid flow and ther- modynamics would be to use the 2-film theory [3–7]. However, use of the surface-renewal theory to couple thermodynamics and fluid flow might not be adequate when slag and metal are mixed, and it certainly would not allow for the study of the mixing itself. Therefore, as a first step towards a process model of a continuous- casting tundish, a model of a tundish built on the basis of fundamental equations, which takes slag, flux and 15 Solhed & Jonsson refractory into account, has been developed and is pre- sented in this paper. Specifically, the model reflects the penetration of the steel and slag phases into each other and other con- ditions at the slag/metal interface. Many authors have studied the dispersion of the slag phase into the steel us- ing physical modelling [8–15]. Among them Kim et al.  determined a critical stirring rate for the break up of the interface in a ladle. From their results it is evi- dent that the interface is fully disintegrated and a mix- ing zone establishes above a certain stirring rate, but it can also be deduced that a certain degree of mixing ex- ists even for low flow rates. Furthermore, Spalding and Villasenor  have shown, using a long duct of rect- angular cross section and 2 fluids of different densities, that the instability that arises because of the presence of shear between the fluid layers will cause a mixing of the layers. They also showed that this instability could be predicted by a fluid-flow calculation, if the position of the interface was calculated. The authors of this paper used these ideas to incorporate the liquid slag phase into their model of a continuous-casting tundish. The predic- tions of heat and fluid flow were validated by compar- ison with both velocity and temperature measurement data from production-scale tundishes. Furthermore, the fluid-flow model including the slag phase has been val- idated by investigation of steel/slag samples taken with a special sampling device . Studying these sam- ples also revealed some information on steel–inclusion interaction. The modelling is described in the section on math- ematical modelling. Thereafter, in the next section, the solution procedure including initial and boundary con- ditions is discussed. The flow and temperature field re- sults are presented in the next section. In a further sec- tion, the slag entrapment results are described as well as the sampling technique, the methods used to inves- tigate the samples and the results of the investigation. Finally, the next sections include a discussion of the pre- sented results, some conclusions and some suggestions on future work. Mathematical modelling The continuous-casting tundish has increasingly evolved into a very useful reactor for steel refining. However, the operating conditions, high temperature and visual opacity of liquid steel make it hard to make direct experimental investigations. Mathematical modelling is a reasonable alternative to investigate fluid-flow and heat-transfer phenomena in continuous- casting tundishes. Today, a large number of modelling efforts covering various aspects such as fluid flow, residence time, inclusion and thermal energy trans- port, etc. have been reported in the literature. These works have led to considerable improvements in our understanding of the various transport processes associated with tundish operations. However, most of the modelling efforts have not included the refractory, slag or flux. Considering refractory, slag and flux in the model should on the one hand render a better prediction of heat and fluid flow, but most importantly make it possible to couple thermodynamic calculations on inclusion chemistry, solidification processes etc. with macro-kinetics derived from first principles. This has been the driving force for the development of the model of a continuous-casting tundish, which besides the steel phase also takes the refractory, slag and flux into account. The basic ideas behind the development of the model are given in the next subsection and the conservation equations in the subsection thereafter. The property variations of the different phases are given in the succeeding subsection, together with the other auxiliary equations and in the last subsection the boundary conditions are stated.